| ||Format||Pages||Price|| |
|PDF Version||5||$42.00||  ADD TO CART|
|Print Version||5||$42.00||  ADD TO CART|
|Standard + Redline PDF Bundle||10||$50.40||  ADD TO CART|
This specification establishes requirements for copper-beryllium alloy seamless tube in straight lengths. The material of manufacture shall be Copper Alloy UNS C17200, cast and worked into tubular form that shall have heat traceable identity. The product shall be manufactured by a combination of hot and cold working, annealing, or precipitation heat treatment, or both, as to produce a uniform wrought structure in the finished product, to meet the temper specified (TB00 (A), TD04 (H), TF00 (AT), or TH04 (HT)). The material shall conform to the chemical composition requirements prescribed for beryllium, copper, aluminum, silicon, and additive elements such as nickel, cobalt, and iron, as determined by chemical analysis. The alloy shall also conform to the specified physical property requirements such as microstructure and grain size, and to the prescribed dimensional and mass requirements. The material shall meet the requirements specified for mechanical properties before and after precipitation heat treatment, such as Rockwell hardness, tensile strength, yield strength, and elongation. Requirements for tension test and other tests to be used to determine the properties mentioned including sampling and specimen preparation are detailed.
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification establishes requirements for copper-beryllium alloy seamless tube in straight lengths. Copper Alloy UNS C17200 will be the alloy furnished whenever Specification B643 is specified.
1.2 Units—The values stated in inch-pound units are to be regarded as standard. The values given in parentheses are mathematical conversions to SI units that are provided for information only and are not considered standard.
1.3 The following safety hazard caveat pertains only to the test methods described in this specification.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
B194 Specification for Copper-Beryllium Alloy Plate, Sheet, Strip, and Rolled Bar
B251 Specification for General Requirements for Wrought Seamless Copper and Copper-Alloy Tube
B601 Classification for Temper Designations for Copper and Copper Alloys--Wrought and Cast
B846 Terminology for Copper and Copper Alloys
E3 Guide for Preparation of Metallographic Specimens
E8/E8M Test Methods for Tension Testing of Metallic Materials
E18 Test Methods for Rockwell Hardness of Metallic Materials
E29 Practice for Using Significant Digits in Test Data to Determine Conformance with Specifications
E112 Test Methods for Determining Average Grain Size
E255 Practice for Sampling Copper and Copper Alloys for the Determination of Chemical Composition
E527 Practice for Numbering Metals and Alloys in the Unified Numbering System (UNS)
ICS Number Code 77.150.30 (Copper products)
UNSPSC Code 40182000(Seamless copper tubes)